ESAB offers a complete line of welding and cutting products and solutions. Explore our equipment offering with ease based on product line and industry.
ESAB is a world leader in welding and cutting equipment and consumables. Explore our complete line of welding & cutting products for virtually every application.
+65 6513 9188
ESAB University Courses are incremental, structured learning modules designed to help you take your skills to the next level. New courses are being added regularly, so please check back often. Click the link to see current courses offered.
Articles cover industry topics more in-depth and are created in partnership with ESAB engineers and master welders. Click the links to see the latest.
Tips from ESAB Experts to help take your welding, cutting and fabrication skills to the next level.
ESAB University videos are curated with tips and best practices from top fabricators around the world. Learn new techniques or improve your current skills with ESAB University videos.
ESAB Welding Handbooks
ESAB Courses are structured learning designed to help welders achieve certain learning milestones and explore topics more in-depth. Check back often for updated resources.
ESAB is a world leader in welding and cutting equipment and consumables. We offer a complete line of fabrication solutions for virtually every application.
ESAB Newsroom - Stay up to date with the latest news from ESAB. View press releases, product announcements, corporate news, and more here.
ESAB EHS (Environment, Health & Safety) initiatives are monitored with the highest degree of importance and commitment to safety is ingrained in our culture.
The history of ESAB is the History of Welding. Go here to view an interactive look at ESAB's history in shaping the future of innovation in welding, cutting, and fabrication.
View available job openings and more on the ESAB Careers page.
ESAB offers a wealth of product support resources, including a range of technical and service publications, from Safety Data Sheets and downloadable product manuals to product certifications.
Visit ESAB's global manual search engine to access the items below and more.
Global User Manuals
Spare Parts List
Product Storage Instructions
View Main Contact Page
View ESAB Location Information
Product Stewardship and Sustainability Inquiry
No Playlist Found ! Please Create Your PlayList Here
Pure aluminum is not usually used for structural applications. To produce aluminum that is of adequate strength for the manufacture of structural components, it is necessary to add other elements to the aluminum. So, what elements can be added to these aluminum alloys? Does adding these elements have any effect on the material’s performance? In what applications are these alloys used?
It would be very unusual to find pure aluminum (1xxx series of alloys) chosen for structural fabrication because of their strength characteristics. Although the 1xxx series are almost pure aluminum, they will respond to strain hardening and especially so if they contain appreciable amounts of impurities such as iron and silicon. However, even in the strain-hardened condition, the 1xxx series alloys have very low strength when compared to the other series of aluminum alloys. When the 1xxx series alloys are chosen for a structural application, they are most often chosen for their superior corrosion resistance and/or their high electrical conductivity. The most common applications for the 1xxx series alloys are aluminum foil, electrical bus bars, metalizing wire, and chemical tanks and piping systems.
The addition of alloying elements to aluminum is the principal method used to produce a selection of different materials that can be used in a wide assortment of structural applications.
If we consider the seven designated aluminum alloy series used for wrought alloys, we can immediately identify the main alloying elements used for producing each of the alloy series. We can then go further and examine each of these elements’ effects on aluminum. We have also added some other commonly used elements and their effects on aluminum.
Copper (Cu) 2xxx –The aluminum-copper alloys typically contain between 2 to 10% copper, with smaller additions of other elements. The copper provides substantial increases in strength and facilitates precipitation hardening. The introduction of copper to aluminum can also reduce ductility and corrosion resistance. The susceptibility to solidification cracking of aluminum-copper alloys is increased. Consequently, some of these alloys can be the most challenging aluminum alloys to weld. These alloys include some of the highest-strength heat treatable aluminum alloys. The most common applications for the 2xxx series alloys are aerospace, military vehicles, and rocket fins.
Manganese (Mn) 3xxx – The addition of manganese to aluminum increases strength somewhat through solution strengthening. It also improves strain hardening while not appreciably reducing ductility or corrosion resistance. These are moderate strength non-heat-treatable materials that retain strength at elevated temperatures and are seldom used for major structural applications. The most common applications for the 3xxx series alloys are cooking utensils, radiators, air conditioning condensers, evaporators, heat exchangers, and associated piping systems.
Silicon (Si) 4xxx –The addition of silicon to aluminum reduces melting temperature and improves fluidity. Silicon alone in aluminum produces a non-heat-treatable alloy. However, in combination with magnesium, it produces a precipitation hardening heat-treatable alloy. Consequently, there are both heat-treatable and non-heat-treatable alloys within the 4xxx series. Silicon additions to aluminum are commonly used for the manufacturing of castings. The most common applications for the 4xxx series alloys are filler wires for fusion welding and brazing of aluminum.
Magnesium (Mg) 5xxx -The addition of magnesium to aluminum increases strength through solid solution strengthening and improves their strain hardening ability. These alloys are the highest strength non-heat-treatable aluminum alloys and are, therefore, used extensively for structural applications. The 5xxx series alloys are produced mainly as sheets and plates and only occasionally as extrusions. The reason for this is that these alloys strain to harden quickly and, are, therefore difficult and expensive to extrude. Some common applications for the 5xxx series alloys are truck and train bodies, buildings, armored vehicles, ship and boat building, chemical tankers, pressure vessels, and cryogenic tanks.
Magnesium and Silicon (Mg2Si) 6xxx – The addition of magnesium and silicon to aluminum produces the compound magnesium-silicide (Mg2Si). The formation of this compound provides the 6xxx series their heat-treatability. The 6xxx series alloys are easily and economically extruded. For this reason, the 6xxx alloys are most often found in an extensive selection of extruded shapes. These alloys form an important complementary system with the 5xxx series alloy. The 5xxx series alloy is used in the form of plates and the 6xxx are often joined to the plate in some extruded form. Some of the common applications for the 6xxx series alloys are handrails, driveshafts, automotive frame sections, bicycle frames, tubular lawn furniture, scaffolding, stiffeners, and braces used on trucks, boats, and many other structural fabrications.
Zinc (Zn) 7xxx –The addition of zinc to aluminum (in conjunction with some other elements, primarily magnesium and/or copper) produces heat-treatable aluminum alloys of the highest strength. The zinc substantially increases strength and permits precipitation hardening. Some of these alloys can be susceptible to stress corrosion cracking and for this reason, are not usually fusion welded. Other alloys within this series are often fusion welded with excellent results. Some of the common applications of the 7xxx series alloys are aerospace, armored vehicles, baseball bats, and bicycle frames.
Iron (Fe) –Iron is the most common impurity found in aluminum and is intentionally added to some pure (1xxx series) alloys to provide a slight increase in strength.
Chromium (Cr) –Chromium is added to aluminum to control grain structure and to prevent grain growth in aluminum-magnesium alloys It also helps prevent recrystallization in aluminum-magnesium-silicon or aluminum-magnesium-zinc alloys during heat treatment. Chromium will also reduce stress corrosion susceptibility and improves toughness.
Nickel (Ni) – Nickel is added to aluminum-copper and aluminum-silicon alloys to improve hardness and strength at elevated temperatures and to reduce the coefficient of expansion.
Titanium (Ti) – Titanium is added to aluminum primarily as a grain refiner. The grain refining effect of titanium is enhanced if boron is present in the melt or if it is added as a master alloy containing boron largely combined as TiB2. Titanium is a common addition to aluminum weld filler wire as it refines the weld structure and helps to prevent weld cracking.
Zirconium (Zr) – Zirconium is added to aluminum to form a fine precipitate of intermetallic particles that inhibit recrystallization.
Lithium (Li) -The addition of lithium to aluminum can substantially increase strength and, Young’s modulus, provide precipitation hardening and decreases density.
Lead (Pb) and Bismuth (Bi) – Lead and bismuth are added to aluminum to assist in chip formation and improve machinability. These free machining alloys are often not weldable because the lead and bismuth produce low melting constituents and can produce poor mechanical properties and/or high crack sensitivity on solidification.
There are many aluminum alloys used in industry today. Over 400 wrought alloys and over 200 casting alloys are currently registered with the Aluminum Association. Certainly, one of the most important considerations encountered during the welding of aluminum is the identification of the aluminum base alloy type to be welded. If the base material type of the component to be welded is not available through a reliable source, it can be difficult to select a suitable welding procedure.
There are some general guidelines as to the most probable type of aluminum used in different applications, such as those mentioned above. However, it is very important to be aware that incorrect assumptions as to the chemistry of an aluminum alloy can result in very serious effects on the weld performance. It is strongly recommended that positive identification of the type of aluminum is made and that welding procedures be developed and tested in order to verify weld performance.